
data_a

_diffrn_radiation_probe  x-ray
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode reflection
_pd_meas_scan_method step
 loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
 1.5406    1.0000
 1.5443    0.5000
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator none

_chemical_name_mineral
;
;

_symmetry_space_group_name_H-M I41/a

_symmetry_cell_setting tetragonal
_symmetry_space_group_name_hall 
;
-I 4ad
;

_cell_length_a  5.242071(96)
_cell_length_b  5.242071(96)
_cell_length_c  11.46775(23)
_cell_angle_alpha 90
_cell_angle_beta  90
_cell_angle_gamma 90
_cell_volume 315.126(13)
_chemical_formula_moiety
;
Er0.07 La0.67 Mo4 O16 Yb0.60, 1.333(Ca Na)
;
_chemical_formula_sum
;
Ca1.33 Er0.07 La0.67 Mo4 Na1.33 O16 Yb0.60
;

_chemical_formula_weight  931.47
_cell_formula_units_Z 1
_exptl_crystal_density_diffrn  4.90808

_exptl_absorpt_coefficient_mu  63.714

_cell_measurement_temperature  300
_diffrn_ambient_temperature  300


_pd_char_colour
;
colourless
;

_cell_measurement_reflns_used 104
_cell_measurement_theta_min 5
_cell_measurement_theta_max 45
_pd_proc_number_of_points 4000
_pd_meas_2theta_range_min 10
_pd_meas_2theta_range_max 90
_pd_meas_2theta_range_inc 0.02

_pd_proc_ls_profile_function PearsonVII
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max  0.01000
_refine_ls_R_I_factor 1.65
_pd_proc_ls_prof_wR_factor 15.061
_pd_proc_ls_prof_R_factor 9.970
_pd_proc_ls_prof_wR_expected 13.493
_refine_ls_goodness_of_fit_all 1.116
loop_
_symmetry_equiv_pos_as_xyz
	'x, y, z'
	'-x, -y, -z'
	'-x, -y+1/2, z'
	'-x+1/2, -y, z+1/2'
	'-x+1/2, -y+1/2, -z+1/2'
	'-y+1/4, x+1/4, -z+1/4'
	'-y+1/4, x-1/4, z-1/4'
	'-y-1/4, x+1/4, z+1/4'
	'-y-1/4, x-1/4, -z-1/4'
	'y+1/4, -x+1/4, z+1/4'
	'y+1/4, -x-1/4, -z-1/4'
	'y-1/4, -x+1/4, -z+1/4'
	'y-1/4, -x-1/4, z-1/4'
	'x, y+1/2, -z'
	'x+1/2, y, -z+1/2'
	'x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Na Na 0 0.25 0.625 0.3333333 0.50(17)
Ca Ca 0 0.25 0.625 0.3333333 0.50(17)
La La 0 0.25 0.625 0.1666667 0.50(17)
Er Er 0 0.25 0.625 0.01666667 0.50(17)
Yb Yb 0 0.25 0.625 0.15 0.50(17)
Mo Mo 0 0.25 0.125 1 0.50(17)
O O 0.2405(20) 0.1019(12) 0.04196(57) 1 0.50(26)

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
Na O 2.4820(89) 4_555
Na O 2.4737(79) 5_555
Ca O 2.4820(89) 4_555
Ca O 2.4737(79) 5_555
La O 2.4820(89) 4_555
La O 2.4737(79) 5_555
Er O 2.4820(89) 4_555
Er O 2.4737(79) 5_555
Yb O 2.4820(89) 4_555
Yb O 2.4737(79) 5_555
Mo O 1.7604(88)  .

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
O Na O 68.59(37) 4_555 5_555
O Na O 73.52(31) 4_555 7_556
O Na O 98.47(29) 4_555 9_556
O Na O 151.4(12) 4_555 13_566
O Na O 76.77(30) 4_555 15_455
O Na O 134.88(73) 4_555 16_455
O Na O 126.9(55) 5_555 7_556
O Na O 78.57(29) 5_555 15_455
O Ca O 68.59(37) 4_555 5_555
O Ca O 73.52(31) 4_555 7_556
O Ca O 98.47(29) 4_555 9_556
O Ca O 151.4(12) 4_555 13_566
O Ca O 76.77(30) 4_555 15_455
O Ca O 134.88(73) 4_555 16_455
O Ca O 126.9(55) 5_555 7_556
O Ca O 78.57(29) 5_555 15_455
O La O 68.59(37) 4_555 5_555
O La O 73.52(31) 4_555 7_556
O La O 98.47(29) 4_555 9_556
O La O 151.4(12) 4_555 13_566
O La O 76.77(30) 4_555 15_455
O La O 134.88(73) 4_555 16_455
O La O 126.9(55) 5_555 7_556
O La O 78.57(29) 5_555 15_455
O Er O 68.59(37) 4_555 5_555
O Er O 73.52(31) 4_555 7_556
O Er O 98.47(29) 4_555 9_556
O Er O 151.4(12) 4_555 13_566
O Er O 76.77(30) 4_555 15_455
O Er O 134.88(73) 4_555 16_455
O Er O 126.9(55) 5_555 7_556
O Er O 78.57(29) 5_555 15_455
O Yb O 68.59(37) 4_555 5_555
O Yb O 73.52(31) 4_555 7_556
O Yb O 98.47(29) 4_555 9_556
O Yb O 151.4(12) 4_555 13_566
O Yb O 76.77(30) 4_555 15_455
O Yb O 134.88(73) 4_555 16_455
O Yb O 126.9(55) 5_555 7_556
O Yb O 78.57(29) 5_555 15_455
O Mo O 114.6(55) 1_555 3_555
O Mo O 107.02(44) 1_555 6_555